Ultralight Metallic Microlattices T. A. Schaedler et al. Science
334, 962 (2011); DOI: 10.1126/science.1211649
This copy is for your personal, non-commercial use only.
If you wish to distribute this article to others, you can order
high-quality copies for your colleagues, clients, or customers by
clicking here. Permission to republish or repurpose articles or
portions of articles can be obtained by following the guidelines
here. The following resources related to this article are available
online at www.sciencemag.org (this information is current as of May
14, 2012 ): Updated information and services, including
high-resolution figures, can be found in the online version of this
Online Material can be found at:
A list of selected additional articles on the Science Web sites
related to this article can be found at:
This article cites 23 articles, 2 of which can be accessed free:
This article appears in the following subject collections:
Materials Science http://www.sciencemag.org/cgi/collection/mat_sci
Downloaded from www.sciencemag.org on May 14, 2012
Science (print ISSN 0036-8075; online ISSN 1095-9203) is
published weekly, except the last week in December, by the American
Association for the Advancement of Science, 1200 New York Avenue
NW, Washington, DC 20005. Copyright 2011 by the American
Association for the Advancement of Science; all rights reserved.
The title Science is a registered trademark of AAAS.
Ultralight Metallic MicrolatticesT. A. Schaedler,1* A. J.
Jacobsen,1 A. Torrents,2 A. E. Sorensen,1 J. Lian,3 J. R. Greer,3
L. Valdevit,2 W. B. Carter1 Ultralight (50% compression while
demonstrating large energy absorption upon cyclic loading. The base
architecture of our metallic microlattices consists of a periodic
array of hollow tubes that connect at nodes, forming an octahedral
unit cell without any lattice members in the basal plane. Figure 1
illustrates how the microlattice architecture can be distilled into
three levels of hierarchy at three distinct length scales: unit
cell (~mm to cm), hollow tube lattice member (~mm to mm), and
hollow tube wall (~nm to mm). Each architectural element can be
controlled independently, providing exceptional control over the
design and properties of the resulting micro-
lattice. The architecture determines the relative density of the
lattice, with the absolute density dictated by the film material.
The fabrication process begins with solid microlattice templates
fabricated by using a selfpropagating photopolymer waveguide
technique. In this method, a thiol-ene liquid photomonomer is
exposed to collimated ultraviolet (UV) light through a patterned
mask, producing an interconnected three-dimensional photopolymer
lattice (11). A wide array of different architectures with unit
cell dimensions ranging from 0.1 to >10 mm can be made by
altering the mask pattern and the angle of the incident light (12,
13). Here, we focus on architectures with 1- to 4-mm lattice member
length L, 100- to 500-mm lattice member diameter D, 100- to 500-nm
wall thickness t, and 60 inclination angle q, similar to the
microlattices depicted in Fig. 1. Conformal nickelphosphorous thin
films were deposited on the polymer lattices by electroless
plating, and the polymer was subsequently etched out (table S1).
The autocatalytic electroless nickel-plating reaction enables
deposition of thin films with controlled thickness on complex
shapes and inside pores without noticeable mass transport
limitations. The ultralight microlattice essentially translates the
deposited nanoscale thin film in three dimensions to form a
macroscopic material where the base structural elements are hollow
tubes. By controlling the reaction time, a 100-nm-thick uniform
conformal coating can be achieved, resulting in a cellular material
with a density of 0.9 mg/cm3 (Fig. 1). The density is calculated by
using the weight of the solid structure but not including the
REPORTSweight of air in the pores, adhering to the standard
practice for cellular materials. The density of air at ambient
conditions, 1.2 mg/cm3, multiplied by its volume fraction would
need to be added to express the density of the solid-air composite.
This method to form microlattices allows significantly more control
than typical methods for forming other ultralightweight materials,
such as foams and aerogels, where nominally random processes govern
porosity formation. Characterization of the base constituent by
transmission electron microscopy (TEM) revealed that as-deposited
electroless nickel thin films have an average grain size of ~7 nm,
which is consistent with literature reports (14, 15).
Energy-dispersive x-ray spectroscopy confirmed that the film
composition is 7% phosphorous and 93% nickel by weight. Because the
films were not annealed after deposition, they remained as a
supersaturated solid solution of phosphorous in a crystalline
face-centered cubic nickel lattice with no Ni3P precipitates
present (14). The 7-nm grain size renders electroless nickel thin
films harder and more brittle than typical nano- and
microcrystalline nickel. A hardness of 6 GPa and a modulus of 210
GPa were measured by nanoindentation and hollow tube compression
experiments, respectively (16). Compression experiments on the
as-formed microlattices showed a nearly complete recovery
Fig. 2. Nickel microlattices exhibit recoverable deformation.
(A) Before deformation. (B) 15% compression. (C) 50% compression.
(D) Full recovery after removal of load. (E) Optical image of unit
cell unloaded. (F) Example of node buckling under compression. (G)
SEM image of node before testing. (H) SEM image of node after six
compression cycles at 50% strain. (The compression test is shown in
Fig. 3. Multicycle compression test results of nickel
microlattices. (A) Stress-strain curves of a microlattice with 14
mg/cm3 exhibiting recoverable deformation (compare with Fig. 2).
(B) History of compressive modulus, yield stress, maximum stress,
and energy loss coefficient during the first six compression cycles
shown in (A). (C) Stress-strain curve of a microlattice with a
density of 1.0 mg/cm3. (D) Stress-strain curves of a microlattice
with 43 mg/cm3 showing deformation more typical for metallic
cellular materials. (E) SEM micrograph of postnanoindentation mark
in 500-nm-thick electroless nickel film demonstrating brittle
18 NOVEMBER 2011
Downloaded from www.sciencemag.org on May 14, 2012
REPORTSfrom strains exceeding 50% (movie S1). Figure 2, A to D,
provides images of a 14 mg/cm3 microlattice sample (L = 1050 mm, D
= 150 mm, t = 500 nm) during compression testing, and Fig. 3A
conveys the corresponding stress-strain curve measured at a
prescribed displacement rate of 10 mm/s. In this experiment, the
sample was not constrained by face sheets or attached to any
compression platens. Because of a small taper in lattice strut
diameter, the deformation typically initiates at a particular
surface. Upon first compression, the lattice exhibits a compressive
modulus of 529 kPa, with deviations from linear elastic behavior
starting at ~10 kPa. The stress decreases slightly after the peak,
which is associated with buckling and node fracture events, and a
broad plateau is subsequently established in the stress-strain
curve as buckling and localized node fracture events spread through
the lattice. Figure 2C shows the microlattice at 50% compression.
Upon unloading, the stress drops rapidly but does not approach zero
until the platen is close to its original position. After removing
the load, the microlattice recovers to 98% of its original height
and resumes its original shape (Figs. 2D and 3A). The stress-strain
behavior corresponding to the first cycle is never repeated during
subsequent testing. Rather, during a second compression, the peak
stress is absent and the pseudohardening behavior changes, but the
stress level achieved at 50% strain is only 10% lower than that
after the first cycle. Consecutive compression cycles exhibit
stress-strain curves nearly identical to those of the second
compression. Stiffness and strength diminish with cycle number but
remain almost constant after the third cycle (Fig. 3B). The
microlattice also shows significant hysteresis during compression
experiments. For the first cycle, we estimate the work done in
compression to be 4.6 mJ/cm3 and the energy dissipation to be 3.5
mJ/cm3, yielding an energy loss coefficient (Du/u) of 0.77. This
large energy dissipation results from extensive node microcracking
and thus is limited to the first cycle. After three cycles, a
nearly constant energy loss coefficient of ~ 0.4 is calculated
(Fig. 3B). From this estimate, we extract a loss coefficient (tan
d) of ~ 0.16 (17), an order of magnitude higher than for typical
nickel foams (18). Figure 3C shows the stress-strain response of a
1.0 mg/cm3 sample with larger unit cells (L = 4 mm, D = 500 mm, t =
120 nm), illustrating that different microlattice architectures in
the ultralow-density regime result in similar behavior [although
this sample underwent an additional freeze-drying process step that
caused some damage (table S1)]. Increasing the density and wall
thickness eventually led to a compression behavior more typical for
metallic cellular materials. Figure 3D shows the stress-strain
curve for a 43-mg/cm3 sample (L = 1050 mm, D = 150 mm, t = 1400
nm), for which recovery upon unloading from 50% strain is
essentially absent. Optical examination of the ultralight
microlattices during deformation suggests that deformation
initiates by local buckling at the nodes (Fig. 2, E and F). A
closer inspection of the microlattices by scanning electron
microscopy (SEM) shows that cracks and wrinkles are introduced
primarily at the nodes during compression (Fig. 2, G and H). This
damage is responsible for the 1 to 2% residual strain observed
after the first compression cycle, as well as for the drop in yield
strength and modulus during subsequent compression cycles. Once
stable relief cracks form at the nodes, the bulk microlattice
material can undergo large effective compressive strains through
extensive rotations about remnant node ligaments, but with
negligible strain in the solid nickel-phosphorous material, thus
requiring no further fracture or plastic deformation. This property
results in the reversible compressive behavior shown in Figs. 2 and
3. The extremely small wall thicknesstodiameter ratio is essential
for this deformation mechanism. Increasing this aspect ratio leads
to excessive fracture and loss of recoverability (Fig. 3D). The
rise in stress at strains of ~40% (Fig. 3A) is a result of
increased interaction between lattice members after localized
compression at the nodes and should not be confused with
densification, which in these samples does not occur until strains
exceed 90% (fig. S2). Similar stress-strain curves as presented in
Fig. 3A are typical for viscoelastic polymer foams (19) and carbon
nanotube forests (20) but not for metal-based materials, implying a
nonconventional loss mechanism is present. Two energy-loss
mechanisms could possibly explain the energy dissipation during
compression cycles: (i) structural damping because of snapping
events (e.g., kinking or local buckling of the trusses) and (ii)
mechanical or Coulomb friction between contacting members (or a
combination of both). This mechanical behavior is especially
unexpected considering the relatively brittle nature of the
constituent electroless nickel thin film, as evidenced by the
formation of cracks near a residual indentation mark (Fig. 3E) and
the rapid collapse upon single hollow truss member compressions
(16). The brittle nature of the film arises from its nanograined
microstructure (~7 nm) that hinders plastic deformation by
dislocation motion (21). However, at the bulk scale microlattices
exhibit completely different properties, because the cellular
architecture effectively transforms this brittle thin film into a
ductile, superelastic lattice by enabling sufficient freedom for
deformation and tolerance to local strains through formation of
stable relief cracks. Plotting the relative compressive modulus,
E/Es, of various fabricated microlattices versus their relative
density, r/rs, shows that the modulus scales with (r/rs)2 (Fig. 4).
This scaling law indicates bending-dominated mechanical behavior
similar to open-cell stochastic foams (8). In contrast, other
materials with densities < 10 mg/cm3, such as aerogels and
carbon nanotube (CNT) foams, exhibit a steeper scaling of E/Es ~
(r/rs)3 (Fig. 4) (22, 23), because of inefficient load transfer
between ligaments. (Incidentally, this also affects the structural
stability of a self-supporting cellular material, imposing a lower
bound on density.) We notice that, although the relative modulus of
topologically designed periodic lattice materials [such as
octet-truss lattices (24)] typically scales linearly with relative
density (25, 26), we do not expect the same scaling for the
microlattices described here because of the absence of struts in
the basal plane (26) and the ultrathin-walled hollow nodes, both of
which facilitate localized bending deformation (Fig. 2F).
Nonetheless, the marked improvement in mechanical efficiency over
any other existing ultralightweight material, achieved by
controlling both dimensions and periodicity of the architecture,
enabled a selfsupporting cellular material with a relative density
an order of magnitude lower than previously realized. Further, by
transforming a brittle Ni-P thin film into a three-dimensional
cellular material and designing a hierarchical cellular
architecture at three Fig. 4. Relative compressive modulus (defined
as the measured Youngs modulus, E, divided by the Youngs modulus of
the constituent solid, Es) of selected cellular materials at low
18 NOVEMBER 2011
Downloaded from www.sciencemag.org on May 14, 2012
REPORTSdistinct length scales, we demonstrated the emergence of
entirely different mechanical properties. In addition to possible
applications for an ultralight material with high energy absorption
and recoverability, we anticipate that these results will help
reshape our understanding of the interaction between material
properties and structural architecture.References and Notes1.
Guinness Book of World Records, Least Dense Solid (2003),
www.guinnessworldrecords.com/records-1/leastdense-solid/. 2. T. M.
Tillotson, L. W. Hrubesh, J. Non-Cryst. Solids 145, 44 (1992). 3.
J. Zou et al., ACS Nano 4, 7293 (2010). 4. A. Verdooren, H. M.
Chan, J. L. Grenestedt, M. P. Harmer, H. S. Caram, J. Am. Ceram.
Soc. 89, 3101 (2006). 5. B. C. Tappan et al., J. Am. Chem. Soc.
128, 6589 (2006). 6. M. Chanda, S. K. Roy, Plastics Technology
Handbook (CRC Press, Boca Raton, FL, 2007). 7. B. A. S. F.
Corporation, Materials Safety Data Sheet for Basotect V3012 (2007),
01_thermoplastics/spe/document/MSDS-Basotect% 20V3012.pdf. 8. L. J.
Gibson, M. F. Ashby, Cellular Solids: Structure and Properties
(Cambridge Univ. Press, Cambridge, 1997). 9. H.-S. Ma, J.-H.
Prvost, R. Jullien, G. W. Scherer, J. Non-Cryst. Solids 285, 216
(2001). 10. R. S. Lakes, Nature 361, 511 (1993). 11. A. J.
Jacobsen, W. Barvosa-Carter, S. Nutt, Acta Mater. 55, 6724 (2007).
12. A. J. Jacobsen, W. Barvosa-Carter, S. Nutt, Adv. Mater. 19,
3892 (2007). 13. A. J. Jacobsen, W. Barvosa-Carter, S. Nutt, Acta
Mater. 56, 2540 (2008). 14. S. H. Park, D. N. Lee, J. Mater. Sci.
23, 1643 (1988). 15. S. Y. Chang, Y. S. Lee, H. L. Hsiao, T. K.
Chang, Metall. Mater. Trans. A 37A, 2939 (2006). 16. J. Lian et
al., Nano Lett. 11, 4118 (2011). 17. G. F. Lee, B. Hartmann, J.
Sound Vibrat. 211, 265 (1998). 18. M. F. Ashby et al., Metal Foams:
A Design Guide (Butterworth-Heinemann, Burlington, MA, 2000), p.
43. 19. N. J. Mills, Cell. Polym. 5, 293 (2006). 20. A. Cao, P. L.
Dickrell, W. G. Sawyer, M. N. Ghasemi-Nejhad, P. M. Ajayan, Science
310, 1307 (2005). 21. J. R. Trelewicz, C. A. Schuh, Acta Mater. 55,
5948 (2007). 22. J. Gross, T. Schlief, J. Fricke, Mater. Sci. Eng.
A 168, 235 (1993). 23. M. A. Worsley, S. O. Kucheyev, J. H. Satcher
Jr., A. V. Hamza, T. F. Baumann, Appl. Phys. Lett. 94, 073115
(2009). 24. V. S. Deshpande, N. A. Fleck, M. F. Ashby, J. Mech.
Phys. Solids 49, 1747 (2001). 25. V. S. Deshpande, M. F. Ashby, N.
A. Fleck, Acta Mater. 49, 1035 (2001). 26. V. S. Deshpande, N. A.
Fleck, Int. J. Solids Struct. 38, 6275 (2001). 27. L. J. Gibson, M.
F. Ashby, Proc. R. Soc. London Ser. A 382, 43 (1982). 28. Hexcel
Corporation, HexWeb Honeycomb Attributes and Properties (1999);
datasheet available at www.hexcel.
Honeycomb_Attributes_and_Properties.pdf. 29. M. Moner-Girona, A.
Roig, E. Molins, E. Martinez, J. Esteve, Appl. Phys. Lett. 75, 653
(1999). Acknowledgments: The authors gratefully acknowledge the
financial support by Defense Advanced Research Projects Agency
under the Materials with Controlled Microstructural Architecture
program managed by J. Goldwasser (contract no. W91CRB-10-0305) and
thank J. W. Hutchinson and C. S. Roper for useful discussions. A
patent application regarding the structure and formation process of
the ultralight microlattices has been submitted to the U.S. Patent
and Trademark Office. The polymer waveguide process has been
patented (U.S. Patent 7,382,959, U.S. Patent 7,653,279, and U.S.
Patent 8,017,193), but the template can be fabricated in other
Supporting Online Material
25 July 2011; accepted 12 October 2011
Silica-Like Malleable Materials from Permanent Organic
NetworksDamien Montarnal, Mathieu Capelot, Fran Tournilhac, Ludwik
Leibler* ois Permanently cross-linked materials have outstanding
mechanical properties and solvent resistance, but they cannot be
processed and reshaped once synthesized. Noncross-linked polymers
and those with reversible cross-links are processable, but they are
soluble. We designed epoxy networks that can rearrange their
topology by exchange reactions without depolymerization and showed
that they are insoluble and processable. Unlike organic compounds
and polymers whose viscosity varies abruptly near the glass
transition, these networks show Arrhenius-like gradual viscosity
variations like those of vitreous silica. Like silica, the
materials can be wrought and welded to make complex objects by
local heating without the use of molds. The concept of a glass made
by reversible topology freezing in epoxy networks can be readily
scaled up for applications and generalized to other chemistries.
hermoset polymers such as Bakelite must be polymerized in a mold
having the shape of the desired object because once the reaction is
completed, the polymer cannot be reshaped or reprocessed by heat or
with solvent. In contrast, thermoplastics, when heated, can flow,
which permits extrusion, injection, and molding of objects.
Depending on the chemical nature of the plastic, during cooling,
solidification occurs by crystallization or by glass transition.
During vitrification, as the temperature is lowered below the glass
transition, the viscosity abruptly in-
Matire Molle et Chimie, UMR 7167 CNRS-ESPCI, Ecole Suprieure de
Physique et Chimie Industrielles, 10 rue Vauquelin, 75005 Paris,
France. *To whom correspondence should be addressed. E-mail:
creases in a narrow temperature range, and the material becomes
so viscous that it behaves essentially like a solid with an elastic
modulus of about 109 to 1010 Pa (1). Nevertheless, compared to
processable plastics, cross-linked polymers have superior
dimensional stability; have high-temperature mechanical, thermal,
and environmental resistance; and are irreplaceable in many
demanding applications, such as in the aircraft industry.
High-performance coatings, adhesives, rubbers, light-emitting diode
lenses, and solar cell encapsulants are made of permanently
cross-linked polymer networks as well. Making covalent links
reversible could provide a way to combine processability,
reparability, and high performance (26). Networks with bonds able
to break and reform (79) or to exchange pairs of atoms (10) can
relax stresses and flow. SCIENCE VOL 334
The challenge is to allow rapid reversible reactions at high
temperatures or by a convenient stimulus and to fix the network at
service conditions. In this context, cleavage or exchange reactions
by addition-fragmentation in the presence of radicals offer
interesting possibilities (5, 1114). Scott et al. demonstrated
photoinduced plasticity in cross-linked polymers (11). Similarly,
reparability and self-healing can be induced either thermally (13)
or photochemically (15, 16) in radical systems. However, these
systems undergo unavoidable termination reactions that limit
reversibility of the networks. In parallel, a completely different
concept based on chemical equilibrium between bond breaking and
reforming without irreversible side reactions has been developed
(1720). In these systems, heating has two effects: It displaces the
equilibrium toward depolymerization and it accelerates the bond
breaking and reforming rate (8, 9). The advantage of such
reversible links is that both above-mentioned effects act together
to bring fluidity and thus processability (5, 1719). They are,
however, detrimental to the network integrity and performance. Chen
et al. have shown that to avoid flow and creep at service
temperatures, one can rely, as in thermoplastics, on glass
transition to quench the system (17). Unfortunately, the systems
based on chemical equilibrium between bond breaking and reforming
are sensitive to solvents because in the presence of a solvent, the
chemical equilibrium is displaced toward network depolymerization
and dissolution (19). We sought to show that reversible networks
can flow while maintaining their integrity and insolubility at high
temperature. The idea is to
18 NOVEMBER 2011
Downloaded from www.sciencemag.org on May 14, 2012
and Methods Fig. S1 Table S1 References Movie S1